17.1 Introduction Sheet metal processes involve plane stress loadings and lower forces than bulk forming Almost all sheet metal forming is considered to be secondary processing The main categories of sheet metal forming are: ◦Shearing ◦Bending ◦Drawing
17.2 Shearing Operations Shearing- mechanical cutting of material without the formation of chips or the use of burning or melting ◦Both cutting blades are straight Curved blades may be used to produce different shapes ◦Blanking ◦Piercing ◦Notching ◦Trimming
Shearing Operations Fracture and tearing begin at the weakest point and proceed progressively or intermittently to the next-weakest location ◦Results in a rough and ragged edge Punch and die must have proper alignment and clearance Sheared edges can be produced that require no further finishing
Figure 17-1 Simple blanking with a punch and die. Shearing Operations
Classification of Metalforming Operations
Types of Shearing Simple shearing- sheets of metal are sheared along a straight line Slitting- lengthwise shearing process that is used to cut coils of sheet metal into several rolls of narrower width Figure 17-5 Method of smooth shearing a rod by putting it into compression during shearing.
Figure 17-2 (Left) (Top) Conventionally sheared surface showing the distinct regions of deformation and fracture and (bottom) magnified view of the sheared edge. (Courtesy of Feintool Equipment Corp., Cincinnati, OH.) Shearing Operations
Piercing and Blanking Piercing and blanking are shearing operations where a part is removed from sheet material by forcing a shaped punch through the sheet and into a shaped die Blanking- the piece being punched out becomes the workpiece Piercing- the punchout is the scrap and the remaining strip is the workpiece Figure 17-8 (Above) (Left to Right) Piercing, lancing, and blanking precede the forming of the final ashtray. The small round holes assist positioning and alignment. Figure 17-7 Schematic showing the difference between piercing and blanking.
Fine Blanking Operations Fine Blanking - the piece being punched out becomes the workpiece and pressure pads are used to smooth edges in shearing Figure 17-3 (Top) Method of obtaining a smooth edge in shearing by using a shaped pressure plate to put the metal into localized compression and a punch and opposing punch descending in unison.
Figure 17-4 Fineblanked surface of the same component as shown in Figure (Courtesy of Feintool Equipment Corp., Cincinnati, OH.) Shearing Operations
Types of Piercing and Blanking Lancing- piercing operation that forms either a line cut or hole Perforating- piercing a large number of closely spaced holes Notching- removes segments from along the edge of an existing product Nibbling- a contour is progressively cut by producing a series of overlapping slits or notches
Sheet-metal Cutting Operations
Types of Piercing and Blanking Cutoff- a punch and a die are used to separate a stamping or other product from a strip of stock
Tools and Dies for Piercing and Blanking Basic components of a piercing and blanking die set are: punch, die, and stripper plate Punches and dies should be properly aligned so that a uniform clearance is maintained around the entire border Punches are normally made from low-distortion or air-hardenable tool steel Figure The basic components of piercing and blanking dies.
Blanking Operations Figure Blanking with a square-faced punch (left) and one containing angular shear (right). Note the difference in maximum force and contact stroke. The total work (the are under the curve) is the same for both processes.
Progressive Die Sets Progressive die sets- two or more sets of punches and dies mounted in tandem Transfer dies move individual parts from operation to operation within a single press Compound dies combine processes sequentially during a single stroke of the ram Figure Progressive piercing and blanking die for making a square washer. Note that the punches are of different length.
Design for Piercing and Blanking Design rules ◦Diameters of pierced holes should not be less than the thickness of the metal with a minimum 0f 0.3 mm (0.025”) ◦Minimum distance between holes or the edge of the stock should be at least equal to the metal thickness ◦The width of any projection or slot should be at least 1 times the metal thickness and never less than 2.5 mm (3/32”) ◦Keep tolerances as large as possible ◦Arrange the pattern of parts on the strip to minimize scrap
Clearance Calculation The recommended clearance is: C = at Where c – clearance, in (mm); a – allowance; and t - stock thickness, in (mm). Allowance a is determined according to type of metal. From Mikell P. Groover “Fundamentals of Modern Manufacturing”.
Design Die and Punch Sizes For a round blank of diameter D b is determined as: Blank punch diameter = D b - 2c Blank die diameter = D b For a round hole (piercing) of diameter D h is determined as: Hole punch diameter = D h Hole die diameter = D b + 2c
Cutting Forces Cutting forces are used to determine size of the press needed. F = StL Where S – shear strength of the sheet metal, lb/in 2 (Mpa); t – sheet thickness in. (mm); and L – length of the cut edge, in. (mm). In blanking, punching, slotting, and similar operations, L is the perimeter length of blank or hole being cut. Note: the equation assumes that the entire cut along sheared edge length is made at the same time. In this case, the cutting force is a maximum.
Angular Clearance for slug or blank to drop through the die, the die opening must have an angular clearance of 0.25 to on each side.
Example for Calculating Clearance and Force Round disk of 3.0” dia. is to be blanked from a half-hard cold-rolled sheet of 1/8” with shear strength = 45,000 lb/in 2. Determine (a) punch and die diameters, and (b) blanking force. (a). From table, a = 0.075, so clearance c = 0.075(0.125) = ”. Die opening diameter = 3.0” Punch diameter = 3 – 2(0.0094) = in (b) Assume the entire perimeter of the part is blanked at one time. L = D b = 3.14(3) = 9.426” F = 45,000(9.426)(0.125) = 53,021 lb = tons
Design Example Figure Method for making a simple washer in a compound piercing and blanking die. Part is blanked (a) and subsequently pierced (b) in the same stroke. The blanking punch contains the die for piercing.
17.3 Bending Bending is the plastic deformation of metals about a linear axis with little or no change in the surface area Forming- multiple bends are made with a single die Drawing and stretching- axes of deformation are not linear or are not independent Springback is the “unbending” that occurs after a metal has been deformed Figure (Top) Nature of a bend in sheet metal showing tension on the outside and compression on the inside. (Bottom) The upper portion of the bend region, viewed from the side, shows how the center portion will thin more than the edges.
Angle Bending (Bar Folder and Press Brake) Bar folders make angle bends up to 150 degrees in sheet metal Press brakes make bends in heavier sheets or more complex bends in thin material Figure Press brake dies can form a variety of angles and contours. (Courtesy of Cincinnati Incorporated, Cincinnati, OH.)
Design for Bending Several factors are important in specifying a bending operation ◦Determine the smallest bend radius that can be formed without cracking the metal ◦Metal ductility ◦Thickness of material Figure Relationship between the minimum bend radius (relative to thickness) and the ductility of the metal being bent (as measured by the reduction in area in a uniaxial tensile test).
Considerations for Bending If the punch radius is large and the bend angle is shallow, large amounts of springback are often encountered The sharper the bend, the more likely the surfaces will be stressed beyond the yield point Figure Bends should be made with the bend axis perpendicular to the rolling direction. When intersecting bends are made, both should be at an angle to the rolling direction, as shown.
Design Considerations Determine the dimensions of a flat blank that will produce a bent part of the desired precision Metal tends to thin when it is bent Figure One method of determining the starting blank size (L) for several bending operations. Due to thinning, the product will lengthen during forming. l 1, l 2, and l 3 are the desired product dimensions. See table to determine D based on size of radius R where t is the stock thickness.
Roll Bending Roll bending is a continuous form of three- point bending ◦Plates, sheets, beams, pipes Figure (Left) Schematic of the roll- bending process; (right) the roll bending of an I-beam section. Note how the material is continuously subjected to three- point bending. (Courtesy of Buffalo Forge Company, Buffalo, NY.)
Draw Bending, Compression Bending, and Press Bending Figure (a) Draw bending, in which the form block rotates; (b) compression bending, in which a moving tool compresses the workpiece against a stationary form; (c) press bending, where the press ram moves the bending form.
Engineering Analysis of Bending Bending radius R is normally specified on the inside of the part, rather than at the neutral axis. The bending radius is determined by the radius on the tooling used for bending. Bending Allowance: If the bend radius is small relative to sheet thickness, the metal tends to stretch during bending. ◦BA = 2A(R + K ba t)/360 ◦Where BA – bend allowance, in. (mm); A - bend angle, degrees; R – bend radius, in. (mm); t – sheet thickness; and K ba - factor to estimate stretching. According to , if R =2t, K ba =0.5.: Hoffman, E.G., Fundamentals of Tool Design, 2 nd ed.
Engineering Analysis of Bending Spring back: When the bending pressure is removed at the end of deformation, elastic energy remains in the bend part, causing it to recover partially toward its original shape. SB = (A’ – A b ’)/A b ’ Where SB – springback; A’ – included angle of sheet-metal part; and A b ’ – included angle of bending tool, degrees. From Mikell P. Groover “Fundamentals of Modern Manufacturing”.
Bending Force: The force required to perform bending depends on the geometry of the punch and die and the strength, thickness, and width of the sheet metal. The maximum bending force can be estimated by means of the following equation based on bending of a simple beam: F = (K bf T S wt 2 )/D Where F – bending force, lb (N),; T S – tensile strength of the sheet metal, lb/in 2. (Mpa); t – sheet thickness, in. (mm); and D – die opening dimension. K bf – a constant that counts for differences in an actual bending processes. For V-bending K bf =1.33, and for edge bending K bf =0.33 Engineering Analysis of Bending
Metal to be bent with a modulus of elasticity E = 30x10 6 lb/in 2., yield strength Y = 40,000lb/in 2, and tensile strength T S = 65,000 lb/in 2. Determine (a) starting blank size, and (b) bending force if V-die will be used with a die opening dimension D = 1.0in. (a) W = 1.75’, and the length of the part is: BA. R/t = 0.187/0.125 = 1.5 < 2.0, so K ba = 0.33 For an included angle A’ = 120 0, then A = 60 0 BA = 2A(R + K ba t)/360 =260( x 0.125)/360 = 0.239” Length of the bank is = 2.739” (b)Force: F = (K bf T S wt 2 )/D = 1.33 (65,000)(1.75)(0.125) 2 /1.0 = 2,364 lb Example for Sheet-metal Bending